Subwavelength FabryPerot resonator: a pair of quantum dots incorporated with gold nanorod
 JiunnWoei Liaw^{1, 2},
 ChunHui Huang^{3},
 BaeRenn Chen^{3} and
 MaoKuen Kuo^{3}Email author
DOI: 10.1186/1556276X7546
© Liaw et al.; licensee Springer. 2012
Received: 23 August 2012
Accepted: 24 September 2012
Published: 2 October 2012
Abstract
The two apexes of an elongated gold nanorod (GNR) irradiated by a plane wave are shown to be the hotspots at the longitudinal plasmon modes. This phenomenon implies that a pair of quantum dots (QDs) located at these apexes might be excited simultaneously if the excitation band of QDs coincides with one of these modes. Consequently, a coherent emission of the two emitters could happen subsequently. In the following coherent emission, these twolevel emitters are simulated as two oscillating dipoles (bidipole) with some possible phase differences. Our results show that the maximum radiative and nonradiative powers of the bidipole occur at the longitudinal plasmon dipole, quadrupole, sextupole, and octupole modes of GNR. Moreover, the strongest emissions are induced by the inphase bidipole coupled to the odd modes and the 180° outofphase one to the even modes, respectively. The excitation and emission behaviors of a pair of QDs incorporated with GNR demonstrate the possibility of using this structure as a subwavelength resonator of FabryPerot type. In addition, the correlation between these modes of the GNR and the dispersion relation of gold nanowire is also discussed.
Keywords
Gold nanorod Quantum dot Longitudinal plasmon mode FabryPerot resonator Radiative power Nonradiative power Gold nanowire BidipoleBackground
Single photon of a quantum dot (QD) coupling with the surface plasmon polaritons of metallic nanowire has attracted wide attentions recently [1–4]. In addition, the dispersion relations of the surface plasmon polaritons (or waves) along gold or silver nanowire [5–9] and the longitudinal plasmon modes of gold or silver nanorods [10, 11] have been studied extensively. The nanoantenna effect and FabryPerot resonator of gold nanorod (GNR) through the longitudinal plasmon modes for the emission of nanoemitters (e.g., QD and molecule) have also been studied in the past decade [12–14]. The correlation between the surface plasmon polaritons of metallic nanowire and the plasmon modes of nanorod is an important pivot in linking the submicron and the nanooptics [15, 16]. Because the lowerorder plasmon modes of an elongated metallic nanorod are within the nearinfrared (NIR) regime [14], it is particularly worth for study. Recently, these longitudinal plasmon modes of nanorods and nanowires have been investigated using the electric energy loss spectroscopy (EELS) [17–20]. Moreover, the plasmonenhanced fluorescence of a fluorophore endlinked to GNR has also been demonstrated [21]. In addition, the excitonplasmon structure of two identical QDs coupling to gold nanoparticle has been studied theoretically [22].
In this paper, the longitudinal plasmon modes of an elongated GNR irradiated by a plane wave will be studied first to illustrate that the apexes of GNR are the hotspots at these modes. This phenomenon implies that a pair of QDs at these areas might be excited simultaneously with the aid of the plasmon modes of GNR. Once the two QDs are excited and start to emit photon coherently, they are modeled as two electric dipoles with a phase difference in our analysis. To clarify the transition roles from metallic nanorod to nanowire, we investigate the plasmonic enhancement of an elongated GNR with a higher aspect ratio (AR), e.g., AR = 8, on the luminescence of nearby QDs. The farfield radiation patterns and the nearfield distributions of the system will be analyzed, particularly at longitudinal plasmon modes of the GNR. In addition, the correlation between these modes and the dispersion relation of a gold nanowire (GNW) will be addressed.
Methods
We assume that the GNR is placed on a glass substrate in air. The effective refractive index of the surrounding medium is denoted by n; n = (1−β) n_{sub} + β n_{air}, where the value of β is taken as 0.5, hence n = 1.25. The permittivity of gold is referred in [23]. Note that the wavelength of light, λ, throughout this paper is referred to that in vacuum; the corresponding wavelength in the surrounding medium is then λ/n. We employed the multiple multipole (MMP) method to analyze the electromagnetic field of the problem, based on the Maxwell’s equations [24, 25].
where S_{c} is the surface of GNR [25, 26].
where J_{0} and J_{1} are Bessel functions of the first kind of order 0 and 1, respectively, and H_{0}^{(1)} and H_{1}^{(1)} are Hankel functions of the first kind of order 0 and 1. Here, ζ_{1} and ζ_{2} are related to the wavenumber k as ${\zeta}_{i}^{2}=\mu {\epsilon}_{i}{\omega}^{2}{k}^{2}$, where ε_{1} and ε_{2} are the permittivity of the surrounding medium and gold, respectively, and μ is the permeability. The complex roots $k={k}^{\prime}+i{k}^{\u2033}$ are found numerically to satisfy Equation 3 under the conditions, ${k}^{\prime}\ge 0$ and $\omega =2\pi \phantom{\rule{0.1em}{0ex}}c/\lambda $, for a given angular frequency $\omega =2\pi \phantom{\rule{0.1em}{0ex}}c/\lambda $, where c is the light speed in vacuum. The phase velocity of the surface plasmon wave in GNW is ${v}_{\text{p}}=\omega /k\text{'}$, and the group velocity ${v}_{\text{g}}=\partial \omega /\partial {k}^{\prime}$.
Results and discussion
Conclusions
Our analysis shows that the two apexes of GNR are hotspots, as an elongated GNR is irradiated by a plane wave at the plasmon modes. The phenomenon can increase the probability of the simultaneous excitation of a pair of QDs at these apexes. Consequently, the coherent emission of the two excited QDs may occur subsequently. They were modeled as two emitters: bidipole with phase difference. The radiative power of the bidipole at the apexes of the GNR shows the efficient nanoantenna effect for the emission of QDs at the first and second longitudinal plasmon modes which correspond to the dipole and quadrupole modes. Because the first and second modes of an elongated GNR are in the NIR regime, these modes can be used for the optical communication. On the other hand, the higherorder modes (e.g. the third and fourth modes) of GNR show the darkmode behavior. Moreover, the odd modes are easily induced by the inphase bidipole, but fully suppressed by the 180° outofphase one. On the contrary, the even modes are induced by the 180° outofphase bidipole, but suppressed by the inphase one. Moreover, the strongest emissions are induced by the inphase bidipole coupled to the odd modes, and the 180° outofphase one to the even modes, respectively. Summarily, the plasmon modes of GNR can enhance the simultaneous excitation and coherent emission of a pair of QDs.
These longitudinal plasmon modes of GNR are tunable by adjusting the AR as well as the permittivity of the surrounding medium. In addition, these modes of GNR are consistent with the dispersion relation of GNW. Our preliminary study shows the possibility of using an elongated GNR associated with two QDs at the ends as a subwavelength FabryPerot resonator [10] and might provide further insights for the nanorod spaser [16, 30] and quantum optics [2, 3]. Our analysis could be useful for the plasmonic applications in a variety of rapidly growing fields, e.g., surface enhanced fluorescence [25, 26, 31–33].
Abbreviations
 ACS:

absorption cross section
 AR:

aspect ratio
 ECS:

extinction cross section
 EELS:

electric energy loss spectroscopy
 GNR:

gold nanorod
 GNW:

gold nanowire
 MMP:

multiple multipole
 NIR:

nearinfrared
 QD:

quantum dot
 SCS:

scattering cross section.
Declarations
Acknowledgments
This work was supported by the National Science Council of Taiwan under grant numbers NSC 992221E182030MY3, NSC 1002221E002041MY2 and Chang Gung Memorial Hospital of Taiwan under grant CMRPD 290042.
Authors’ Affiliations
References
 Fedutik Y, Temnov VV, Schops O, Woggon U, Artemyev MV: Excitonplasmonphoton conversion in plasmonic nanostructures. Phys Rev Lett 2007, 99: 136802.View Article
 Akimov AV, Mukherjee A, Yu CL, Chang DE, Zibrov AS, Hemmer PR, Park H, Lukin MD: Efficient generation of single optical plasmons in metallic nanowires coupled to quantum dots. Nature 2007, 450: 402–406. 10.1038/nature06230View Article
 Kolesov R, Grotz B, Balasubramanian G, Stöhr RJ, Nicolet AAL, Hemmer PR, Jelezko F, Wrachtrup J: Waveparticle duality of single surface plasmon polaritons. Nat Phys 2009, 5: 470–474. 10.1038/nphys1278View Article
 Sanders AW, Routenberg DA, Wiley BJ, Xia Y, Dufresne ER, Reed MA: Observation of plasmon propagation, redirection, and fanout in silver nanowires. Nano Lett 2006, 6: 1822–1826. 10.1021/nl052471vView Article
 Schider G, Krenn JR, Hohenau A, Ditlbacher H, Leitner A, Aussenegg FR, Schaich WL, Puscasu I, Monacelli B, Boreman G: Plasmon dispersion relation of Au and Ag nanowires. Phys Rev B 2003, 68: 155427.View Article
 Ditlbacher H, Hohenau A, Wagner D, Kreibig U, Rogers M, Hofer F, Aussenegg FR, Krenn JR: Silver nanowires as surface plasmon resonators. Phys Rev Lett 2005, 95: 257403.View Article
 Wild B, Cao L, Sun Y, Khanal BP, Zubarev ER, Gray SK, Scherer NF, Pelton M: Propagation lengths and group velocities of plasmons in chemically synthesized gold and silver nanowires. ACS Nano 2012, 6: 472–482. 10.1021/nn203802eView Article
 Encina ER, Perassi EM, Coronado EA: Nearfield enhancement of multipole plasmon resonances in Ag and Au nanowires. J Phys Chem A 2009, 113: 4489–4497. 10.1021/jp811089aView Article
 Shegai T, Huang Y, Xu H, Käll M: Coloring fluorescence emission with silver nanowires. Appl Phys Lett 2010, 96: 103114. 10.1063/1.3355545View Article
 Cubukcu E, Capasso F: Optical nanorod antennas as dispersive onedimensional FabryPérot resonators for surface plasmons. Appl Phys Lett 2009, 95: 201101. 10.1063/1.3262947View Article
 Bok HM, Shuford KL, Kim S, Kim SK, Park S: Multiple surface plasmon modes for a colloidal solution of nanoporous gold nanorods and their comparison to smooth gold nanorods. Nano Lett 2008, 8: 2265–2270. 10.1021/nl800924rView Article
 Chau YF, Chen MW, Tsai DP: Threedimensional analysis of surface plasmon resonance modes on a gold nanorod. Appl Opt 2009, 48: 617–622. 10.1364/AO.48.000617View Article
 Yang ZJ, Zhang ZS, Zhang LH, Li QQ, Hao ZH, Wang QQ: Fano resonances in dipolequadrupole plasmon coupling nanorod dimers. Opt Lett 2011, 36: 1542–1544. 10.1364/OL.36.001542View Article
 Biagioni P, Huang JS, Hecht B: Nanoantennas for visible and infrared radiation. Rep Prog Phys 2012, 75: 024402. 10.1088/00344885/75/2/024402View Article
 Dorfmuller J, Vogelgesang R, Khunsin W, Rockstuhl C, Etrich C, Kern K: Plasmonic nanowire antennas: experiment, simulation and theory. Nano Lett 2010, 10: 3596–3603. 10.1021/nl101921yView Article
 Taminiau TH, Stefani FD, van Hulst NF: Optical nanorod antennas modeled as cavities for dipolar emitters: evolution of sub and superradiant modes. Nano Lett 2011, 11: 1020–1024. 10.1021/nl103828nView Article
 Schaffer B, Hohenester U, Trügler A, Hofer F: Highresolution surface plasmon imaging of gold nanoparticles by energyfiltered transmission electron microscopy. Phys Rev B 2009, 79: 041401.View Article
 N'Gom M, Ringnalda J, Mansfield JF, Agarwal A, Kotov N, Zaluzec NJ, Norris TB: Single particle plasmon spectroscopy of silver nanowires and gold nanorods. Nano Lett 2008, 8: 3200–3204. 10.1021/nl801504vView Article
 Nicoletti O, Wubs M, Mortensen NA, Sigle W, van Aken PA, Midgley PA: Surface plasmon modes of a single silver nanorod: an electron energy loss study. Opt Express 2011, 19: 15371–15379. 10.1364/OE.19.015371View Article
 Rossouw D, Couillard M, Vickery J, Kumacheva E, Botton GA: Multipolar plasmonic resonances in silver nanowire antennas imaged with a subnanometer electron probe. Nano Lett 2011, 11: 1499–1504. 10.1021/nl200634wView Article
 Fu Y, Zhang J, Lakowicz JR: Plasmonenhanced fluorescence from single fluorophores endlinked to gold nanorods. J Am Chem Soc 2010, 132: 5540–5541. 10.1021/ja9096237View Article
 He Y, Zhu KD: Strong coupling among semiconductor quantum dots induced by a metal nanoparticle. Nano Res Lett 2012, 7: 95. 10.1186/1556276X795View Article
 Johnson PB, Christy RW: Optical constants of the noble metals. Phys Rev B 1972, 6: 4370–4379. 10.1103/PhysRevB.6.4370View Article
 Hafner C: The Generalized Multipole Technique for Computational Electromagnetics. Boston: Artech House; 1991.
 Liaw JW, Tsai HY: Theoretical investigation of plasmonic enhancement of silicacoated gold nanorod on molecular fluorescence. J Quant Spectrosc Radiat Transfer 2012, 113: 470–479. 10.1016/j.jqsrt.2011.12.015View Article
 Liaw JW, Tsai HY, Huang CH: Sizedependent surface enhanced fluorescence of gold nanorod: enhancement or quenching. Plasmonics 2012, 7(3):543–553. 10.1007/s1146801293419View Article
 Stratton JA: Electromagnetic Theory. New York: McGrawHill; 1941.
 Takahara J, Yamagishi S, Taki H, Morimoto A, Kobayashi T: Guiding of a onedimensional optical beam with nanometer diameter. Opt Lett 1997, 22: 475–477. 10.1364/OL.22.000475View Article
 Liaw JW, Wang JK: Dispersion relation of plasmon wave in metallic nanowires. Scanning 2004, 26: 106–108.
 Bergman DJ, Stockman MI: Surface plasmon amplification by stimulated emission of radiation: quantum generation of coherent surface plasmons in nanosystems. Phys Rev Lett 2003, 90: 027402.View Article
 Wu J, Mangham SC, Reddy VR, Manasreh MO, Weaver BD: Surface plasmon enhanced intermediate band based quantum dots solar cell. Sol Energy Mater Sol Cells 2012, 102: 44–49.View Article
 Long M, Jiang J, Li Y, Cao R, Zhang L, Cai W: Effect of gold nanoparticles on the photocatalytic and photoelectrochemical performance of Au modified BiVO4. NanoMicro Lett 2011, 3(3):171–177.View Article
 Shrivastava S, Dash D: Labelfree colorimetric estimation of proteins using nanoparticles of silver. NanoMicro Lett 2010, 2: 164–168.View Article
Copyright
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.